(2) Par Xuan-Anh TON. Fiber optic chemical sensors based on molecularly imprinted polymers for the detection of mycotoxins. Thèse présentée pour l’obtention du grade de Docteur de l’UTC. Soutenue le 25 octobre 2013 Spécialité : Biotechnologie D2103.
(3) Ce projet est co-financé par l’Union Européenne. L’Europe s’engage en Picardie avec le Fonds européen de développement régional.. DOCTORAL THESIS submitted for graduation as. DOCTEUR de l’Université de Technologie de Compiègne Field: Biotechnology. by. Xuan-Anh TON. Fiber Optic Chemical Sensors Based on Molecularly Imprinted Polymers for the Detection of Mycotoxins Thesis supervised by Prof. Karsten HAUPT and Dr. Bernadette TSE SUM BUI. th. Disputation on 25 October 2013, in front of the jury composed of: ! Chris ALLENDER, Dr.. Cardiff University, United Kingdom. Reviewer. ! Wolfgang KNOLL, Prof.. Austrian Institute of Technology, Austria. Reviewer. ! Daniel THOMAS, Prof.. Université de Technologie de Compiègne, France. President. ! Victor ACHA, Dr.. Institut LaSalle Beauvais, France. Examiner. ! Bernadette TSE SUM BUI, Dr. Université de Technologie de Compiègne, France. Supervisor. ! Karsten HAUPT, Prof.. Supervisor. Université de Technologie de Compiègne, France.
(5) “ Là où est la Volonté est le Chemin.”. !. i.
(6) !. ii.
(7) Acknowledgments!! First&of&all,&I&gratefully&acknowledge&Dr.&Chris&Allender&and&Prof.&Wolfgang&Knoll&for&giving&me&the& honor& to& review& this& thesis,& as& well& as& Prof.& Daniel& Thomas& and& Dr.& Victor& Acha& for& being& the& examiners&of&this&work.& & My& biggest& acknowledgments& go& to& my& supervisors& Prof.& Karsten& Haupt& and& Dr.& Bernadette& Tse& Sum&Bui,&for&their&guidance&during&these&challenging&three&years,&their&constant&availability&and& their&confidence&in&this&project&and&in&me.& Karsten,&first,&thank&you&for&giving&me&the&chance&to&work&on&this&project.&Throughout&these&three& years,& thank& you& for& your& expertise,& your& enthusiasm& and& all& your& creative& ideas& that& built& this& thesis.& Personally,& warm& thanks& for& your& pleasant& company,& your& humor& and& your& openJ mindedness.&It&has&been&a&real&pleasure&to&work&and&interact&with&you.&& Bernadette,&thank&you&for&your&professionalism,&your&constant&support&and&your&numerous&advice,& ideas&and&encouragements.&Above&all,&thanks&for&sharing&your&experience&with&me;&you&taught&me& a& lot& about& the& research& world.& Besides& work,& deep& thanks& for& your& attentiveness,& your& kindness& and&your&good&mood.& ! As&for&our&external&collaborators,&I&am&very&grateful&to&Dr.&Olivier&Soppera,&for&kindly&welcoming& me& in& IS2M,& and& for& his& precious& help& and& his& deep& interest& in& my& work,& as& well& as& Dr.& Arnaud& Spangenberg&and&Ihab&Dika&for&the&nice&collaboration.&I&am&also&thankful&to&Dr.&Marina&Resmini& and& Dr.& Paolo& Bonomi& for& their& contribution& to& this& project,& and& to& Dr.& Victor& Acha& for& the& coordination& of& this& project& to& the& Région& Picardie.& I& gratefully& thank& Dr.& JeanJFrançois& Masson& from& Montréal& University& for& the& nice& collaboration.& Also,& thanks& to& Frédéric& Nadaud& from& the& PhysicoJChemical&Analysis&Unit&of&UTC&for&his&efficiency.&To&finish,&warm&thanks&to&C.D.&Tôn,&Diego& Ros&and&Jérôme&Istria&for&their&personal&implication&and&their&very&valuable&contribution.& & I& sincerely& thank& all& the& members& of& the& Enzyme& and& Cell& Engineering& Laboratory& for& their& sympathy,& their& help,& and& the& friendly& working& environment.& Above& all,& I& especially& thank& the& “Karsten’s& Dream& Team”:& the& MIP& group,& former& or& present& members:& Aude,& Pinar,& Jacqueline,& Serena,& Amani,& Selim,& Zeynep,& Yi,& Paolo,& Marcos…Thanks& also& to& the& nonJimprinted& people:& Thierry,&Jean,&Sébastien,&Melody…&Special&thanks&to&Sofia,&Maria&and&Jingjing,&who&contributed&to& this&work.&To&finish,&very&warm&thanks&to&my&“coffeeJmates”,&the&first&generation,&Yannick,&Carlo& and& Li& Bin,& and& the& second& (German)& generation,& Stephanie& and& Jan,& for& the& very& nice& company& and& the& numerous& exchanges& (scientific& or& not).& For& all& of& you,& thank& you& for& making& my& life& in& Compiègne&so&enjoyable&and&lively!&& & I&will&conclude&these&acknowledgements&for&my&dearest&relatives.&First,&warm&thanks&to&Nelly&and& Gérard& for& the& nice& company.& Among& my& close& friends,& I& especially& thank& Diane& and& Marion& for& their&lovely&friendship.&Very&special&thanks&to&you,&Jarek,&for&being&here&during&these&(difficult)&last& months.& To& finish,& the& most& important& thanks& go& to& my& family,& my& grandJmother& and& my& aunts& Thanh,& Mai& and& Yen& for& their& constant& and& kind& support,& and& finally& my& father& for& his& unique& guidance,& and& my& mother,& my& sister& AnhJChi& and& my& brother& AnhJKiet,& for& their& unconditional& love,&support&and&patience.&&. !. iii.
(8) Abstract1 in1 English:1 Fiber1 optic1 chemical1 sensors1 based1 on1 molecularly1imprinted1polymers1for1the1detection1of1mycotoxins1 Keywords: molecularly imprinted polymer, synthetic receptor, biomimetic sensor, optical fiber, fluorescence, photostructuring. This thesis describes the development of highly selective fiber optic sensors using molecularly imprinted polymers (MIPs) as recognition elements associated with fluorescence for detection. Additionally, we extended the study to the development of other MIP-based optical sensors and sensing methods. MIPs are synthetic biomimetic receptors possessing specific cavities designed for a target molecule. Produced by a templating process at the molecular level, MIPs are capable of recognizing and binding target molecules with selectivities and affinities comparable to those of natural receptors. Compared to biological recognition elements, MIPs are more stable, cheaper and easier to integrate into standard industrial fabrication processes. Hence, MIPs have become interesting alternatives to biomolecules as recognition elements for biosensing. In the first part of this thesis (Chapter 2), MIPs were synthesized by in-situ laser-induced photopolymerization in only a few seconds, as a micrometer-sized tip at the extremity of a telecommunication optical fiber. Photonic and physico-chemical parameters were optimized to tailor the properties of the polymer micro-objects. Gold nanoparticles were incorporated into the MIP microtip for signal enhancement. To prove the efficiency of the sensor, initial studies were performed with a MIP templated with N-carbobenzyloxy-L-phenylalanine (Z-L-Phe) and the fluorescent amino acid derivative dansyl-L-phenylalanine as analyte. The fluorescence was collected either externally at the tip level by an optical fiber connected to a spectrofluorimeter or by collection of the fluorescent signal re-emitted into the fiber through the second arm of a Y-shaped bifurcated fiber. The fluorescent analyte could be detected in the low nM concentrations. In order to monitor nonfluorescent analytes, a naphthalimide-based fluorescent monomer was incorporated into the MIP during its synthesis; fluorescence enhancement was observed when analyte binding occurs. Using this system, the sensor containing a MIP specific for the herbicide 2,4-dichlorophenoxyacetic acid (2,4-D), could detect and quantify this analyte at concentrations as low as 2.5 nM. The signaling MIP-based sensor was also applied to analytes of interest for food safety and biomedical applications, such as the mycotoxin citrinin and the sphingolipid, D-erythro-sphingosine-1-phosphate. In the second part of the thesis (Chapter 3), a different type of fiber optic sensor: cheap, fast and made for “single-use”, was developed by using 4-cm long disposable polystyrene evanescent wave optical fiber waveguides. The coating of the MIP was either performed ex-situ, by dip-coating the fiber in a suspension of MIP particles synthesized beforehand, or in-situ by evanescent-wave photopolymerization directly on the fiber. The resulting fiber optic sensor could detect 2,4-D in the low nM range and demonstrated specific and selective recognition of the herbicide over its structural analogues and other non-related carboxyl-containing analytes. Additionally, we demonstrated the versatility of the system by applying the evanescent wave fiber optic sensor to detect citrinin, a mycotoxin, by simply coating the waveguide with a MIP specific for citrinin. This type of technology could possibly be extended to detect other carboxyl-containing analytes, as long as a specific MIP for the concerned analyte is available. In parallel, the technique of evanescent-wave photopolymerization was used for the synthesis of signaling MIP microdots on continuous and nanostructured gold films. This study lays the foundations for future development of plasmonic MIP nanosensors and microchips. In the last part of the thesis (Chapter 4), an innovative sensing method, based on the use of MIPs and analysis by fluorescence polarization, was developed in order to allow the fast and direct quantification of analytes in food and environmental samples This technique was successfully applied to detect fluoroquinolone antibiotics in tap water and milk, below their maximum residue limits. We can conclude from these studies that we have opened a new era towards the development of a new generation of miniaturized portable MIP-based optical sensors, suitable for on-site measurements and real-time monitoring of environmental and biological analytes in complex media.. !. iv.
(9) Résumé1 en1 Français:1 Capteurs1chimiques1à1fibres1optiques1utilisant1les1 polymères1à1empreintes1moléculaires1pour1la1détection1de1mycotoxines1 Mots-clés: polymère à empreinte moléculaire, récepteur synthétique, capteur biomimétique, fibre optique, fluorescence, photostructuration. Cette thèse décrit le développement de capteurs à fibre optique hautement sélectifs, utilisant des polymères à empreintes moléculaires (MIPs, de l’anglais molecularly imprinted polymers) comme éléments de reconnaissance, et se basant sur la fluorescence pour la détection. Nous avons étendu l’étude à d’autres types de capteurs et de méthodes de détection optiques, toujours basés sur les MIPs. Les MIPs sont des récepteurs synthétiques biomimétiques possédant des cavités spécifiques pour une molécule cible. Produits par un processus de moulage à l’échelle moléculaire, les MIPs sont capables de reconnaître et de se lier à leurs molécules cibles, avec des spécificités et affinités comparables aux récepteurs naturels. De plus, comparé aux récepteurs biologiques, les MIPs sont plus stables, moins chers et plus faciles à intégrer dans les procédés standard industriels de fabrication. Ainsi, les MIPs apparaissent comme une alternative intéressante aux biomolécules en tant qu’éléments de reconnaissance dans les biocapteurs. Dans la première partie de la thèse (Chapitre 2), les MIPs ont été synthétisés en tant que micropointe à l’extrémité d’une fibre optique, par polymérisation in-situ induite par un laser en seulement quelques secondes. Les paramètres photoniques et physico-chimiques ont été optimisés pour moduler les propriétés des micro-objets de polymères. Des nanoparticules d’or ont été incorporées dans la micropointe de MIP afin d’induire une exaltation du signal. Afin de prouver l’efficacité de notre capteur, les études initiales ont été réalisées avec un MIP synthétisé avec le Ncarbobenzyloxy-L-phenylalanine (Z-L-Phe) comme template et le dérivé d’acide aminé fluorescent dansyl-L-phenylalanine, comme analyte. La fluorescence a été collectée de l’extérieur au niveau de la micropointe par une fibre optique connectée à un spectrofluorimètre, ou par collection du signal fluorescent ré-émis dans l’un des bras d’une fibre bifurquée en Y. L’analyte fluorescent a pu être détecté à des concentrations de l’ordre du nM. Afin de quantifier les analytes non fluorescents, un monomère fluorescent, possédant un groupe naphthalimide, a été incorporé dans le MIP ; celui-çi déployant une augmentation de la fluorescence quand l’analyte se lie. Utilisant ce système avec un MIP spécifique pour l’herbicide 2,4-D (acide 2,4-dichlorophénoxyacétique), des concentrations aussi basses que 2,5 nM en 2,4-D ont pu être mesurées. Le capteur MIP a également été appliqué à des analytes d’intérêt pour la sécurité alimentaire et le domaine biomédical, comme la mycotoxine citrinine et le sphingolipide, D-erythro-sphingosine-1-phosphate. Dans la seconde partie (Chapitre 3), un autre type de capteur à fibre optique, en polystyrène, peu cher, rapide et “à usage unique”, a été développé en utilisant des guides d’ondes à ondes évanescentes. Le dépôt du MIP, contenant un monomère rapporteur de fluorescence, est réalisé soit ex-situ, en plongeant la fibre optique dans une suspension de particules de MIPs synthétisées préalablement, ou in-situ par photopolymérisation par onde évanescente directement sur la fibre. Le capteur a été appliqué pour la détection du 2,4-D et de la citrinine. En parallèle, la technique de photopolymérisation par ondes évanescentes a été utilisée pour la synthèse de microdots de MIPs rapporteurs de fluorescence, sur des films d’or et des surfaces d’or nanostructurées. Cette étude pose les bases pour le développement futur de nanocapteurs et de micropuces de MIPs plasmoniques. Dans la dernière partie (Chapitre 4), une méthode d’analyse novatrice, basée sur l’utilisation des MIPs et l’analyse par polarisation de fluorescence, a été développée en vue de permettre la quantification directe et rapide d’analytes dans des échantillons alimentaires et environnementaux. Cette technique a été appliquée avec succès pour détecter des antibiotiques fluoroquinolones dans l’eau du robinet et le lait, en-dessous de leur limite maximale de résidus. En conclusion, nous pouvons dire que ce travail ouvre la voie vers l’application d’une nouvelle génération de capteurs optiques portables, robustes et miniaturisables basés sur les MIPs, pour des mesures «sur-site » et la quantification en temps réel d’analytes biologiques et environnementaux dans des milieux complexes.. !. v.
(10) Table1of1Contents1 Acknowledgements......................................................................................................................iii. Abstract.in.English:.Fiber.optic.chemical.sensors.based.on.molecularly.imprinted. polymers.for.the.detection.of.mycotoxins.............................................................................iv. Résumé.en.Français:.Capteurs.chimiques.à.fibres.optiques.utilisant.les. polymères.à.empreintes.moléculaires.pour.la.détection.de.mycotoxines..................v. List.of.Abbreviations...................................................................................................................vii. General.Introduction.....................................................................................................................1. !. Chapter( 1:. Molecularly. Imprinted. Polymers. and. Their. Applications. in. Optical. Sensing.–.A(Literature(Review…………………………………………………………………………………4. I.. II.. !. Molecular imprinting. 6. I.1. The origin of molecular imprinting. 6. I.2. Fundamentals of molecularly imprinted polymers. 9. I.2.1. The covalent approach. 9. I.2.2. The non-covalent approach based on self-assembly. 9. I.2.3. The 'semi-covalent' approach. 15. I.2.4. Polymerization procedures for MIPs. 17. I.3. Some applications of MIPs. 20. I.3.1. Separation. 20. I.3.2. Binding assays. 21. I.3.3. Drug delivery. 22. I.3.4. Sensors. 22. Application of MIPs in opto-chemical sensors. 23. II.1. Chemical sensors: definition and classification. 23. II.2. Surface Plasmon Resonance. 26. II.2. Surface Enhanced Raman Scattering. 28. II.3. Fluorescence-based MIP optical sensors. 30. II.3.1. Introduction on fluorescence-based molecular sensors. 30. II.3.2. Fluorescent analytes. 31. II.3.3. Competitive and displacement assays. 33. II.3.4. Fluorescence generated by the polymer. 34. vi.
(11) !. .. Table of Contents. . .. II.3.5. Quantum dot photoluminescence. 38. II.4. Molecularly imprinted photonic polymers. 39. II.5. Other MIP-based optical sensors. 41. III.. Conclusions. 45. IV.. References. 45. .. Chapter( 2:. A. fluorescence. fiber. optic. sensor. based. on. in5situ. polymerized. molecularly.imprinted.microstructures……………………………………………………………56. I.. Introduction. 58. II.. Materials and methods. 62. II.1. Reagents and materials. 62. II.2. MIP microtip fabrication process. 64. II.3. Formulations of MIPs. 65. II.4. Preparation of bulk polymers. 66. II.5. Fluorescence emission decay measurements. 66. II.6. Preparation of the MIP P3 by precipitation polymerization. 66. II.7. Binding studies of polymer microtips with the simple fiber. 66. II.7.1. Plain microtip – analyte: dansyl-L-Phe. 66. II.7.2. Core-shell microtip P2 – Analyte: 2,4-D. 67. II.8. Binding studies of polymer microtips on the bifurcated fibers. 67. II.8.1. The bifurcated single-mode fiber. 67. II.8.2. The multimode bifurcated fiber. 67. II.9. Batch binding studies with MIP particles P3. 67. II.10. Synthesis and characterization of the fluorescent monomer “FlM” N-(2-(6-(4methylpiperazin-1-yl)-1,3-dioxo-1H-benzo[de]isoquinolin-2(3H)-yl-ethyl)acrylamide 68 II.11. Synthesis and characterization of the Aushell-Agcore bimetallic nanoparticles. III.. !. 70. II.11.1. Synthesis of the monometallic gold nanoparticles. 70. II.11.2. Synthesis of the silver shell on the gold core. 70. II.11.3. Characterization of the Aushell-Agcore nanoparticles. 70. Results and discussion. 74. III.1. Studies with the simple single-mode fiber (SMF) set-up. 74. III.1.1. Optimization of the MIP formulation and tailoring of the tip geometry. 74. III.1.2. Molecular recognition properties of the imprinted bulk polymers. 76. III.1.3. Effect of photonic parameters on the morphology of polymer microtips. 77. vii.
(12) !. .. Table of Contents. . .. III.1.4. Molecular recognition properties of the MIP microtip. 79. III.1.5. Composite gold nanoparticle-MIP microtip for enhanced sensitivity. 82. III.1.6. A core-shell format of the MIP microtip for a better response time. 87. III.1.7. An intrinsically fluorescent MIP fiber optic probe based on a fluorescent monomer. 88. III.1.8. Conclusions. 94. III.2. The bifurcated SMF set-up (telecom fiber). 95. III.2.1. Molecular recognition properties of the MIP microtip. 95. III.2.2. Composite gold nanoparticle-MIP microtip for an enhanced sensitivity. 96. III.2.3. Conclusions. 99. III.3. Sensing with a bifurcated multimode fiber and a fluorescent signaling MIP microtip. 100. III.3.1. Sensing of the mycotoxin citrinin. 101. III.3.2. Sensing of the sphingolipid D-erythro-sphingosine-1-phosphate. 102. IV.. Conclusions and perspectives. 105. V.. References. 107. Chapter(3:.Synthesis.of.molecularly.imprinted.polymerTcoated.sensing.elements. by.evanescent.wave.photopolymerization.and.topTdown.deposition……………...110. I.. II.. Introduction. 112. I.1. Evanescent-wave fiber optic sensors. 112. I.2. Photopolymerization by evanescent waves. 114. Materials and methods. 117. II.1. Reagents and materials. 117. II.2. Synthesis and characterization of the fluorescent monomer “FlM” N-(2-(6-4methylpiperazin-1-yl)-1,3-dioxo-1H-benzo[de]isoquinolin-2(3H)-yl-ethyl)acrylamide 116 II.3. Preparation of the molecularly imprinted polymers (MIPs) by precipitation polymerization. 117. II.4. Binding studies with the 2,4-D MIP P3. 118. II.5. Binding studies of the citrinin MIPs P-CIT1 and P-CIT2. 118. II.6. Coating of the MIP particles P3 or P-CIT2 on the polystyrene optical waveguides and binding studies. 118. II.7. In-situ polymerization of the MIP on the fiber optic waveguides. 119. II.8. Fabrication of ultra-thin MIP microdots by evanescent-wave polymerization. 119. II.9. Analysis of ultra-thin MIP microdots. 120. II.9.1. Characterization. !. 120. viii.
(13) !. .. Table of Contents. . .. II.9.2. Analyte adsorption tests. III.. 120. Results and discussion. 121. III.1. Sensing of biological and environmental analytes using an evanescent wave fiber optic waveguide coated with a signaling naphtalimide-based imprinted polymer. 121. III.1.1. Sensing of 2,4-D. 121. III.1.2. Sensing of the mycotoxin citrinin. 128. III.1.3. Application of the fluorescent monomer FlM for the recognition of phosphate and sulfate analytes. 132. III.1.4. Conclusions. 134. III.2. Ultra-thin MIP microdots obtained by evanescent-wave polymerization – Synthesis on nanostructured gold surfaces.. 135. III.2.1. Context. 135. II.2.2. Polymerization of the microdots by evanescent waves. 135. II.2.3. Morphology of the polymer microdots. 136. II.2.4. Molecular recognition properties of the polymer microdots. 139. IV.. Conclusions and perspectives. 141. V.. References. 142. Chapter(4:.Direct.fluorimetric.sensing.of.UVTexcited.analytes.in.complex.samples. using. molecularly. imprinted. polymer. nanoparticles. and. fluorescence. polarization………………………………………………………………...…………………………………..144. I.. II.. III.. !. Introduction. 146. I.1. Fluorescence polarization immunoassays (FPIA). 146. I.1.1. Principles of fluorescence polarization and introduction to FPIA. 146. I.1.2. Applications of FPIA. 148. I.2. Molecularly imprinted polymers for the detection of fluoroquinolones. 149. Materials and methods. 152. II.1. Reagents and materials. 152. II.2. Preparation of polymers. 152. II.3. Evaluation of the binding properties of the polymers. 152. II.4. Screening of fluoroquinolones using fluorescence polarization. 153. II.5. Water and milk samples analysis. 153. II.6. Fluorescence emission decay measurements. 153. Results and discussion. 155. III.1. Synthesis and characterization of the polymers. 155. ix.
(14) !. .. Table of Contents. . .. III.2. Fluorescence polarization measurements. 158. III.3. Application of fluorescence polarization to measure ENRO in buffer media and in tap water. 163. III.4. Application of fluorescence polarization to measure ENRO and FQs in milk. 164. IV.. Conclusions. 167. V.. References. 168. General.Conclusions.and.Perspectives…………………………………………………………….172. Annex:.Achievements………………………………………………………………………………………174.. !. x.
(15) !. List1of1Abbreviations1 ABDV ACN AcOH AFM AIBN AMP AMPI CCD CIPRO CMMC CP 2,4-D DANO Dansyl-Phe DVB 2,4-D-OMe. azo-bis-dimethylvaleronitrile acetonitrile acetic acid atomic force microscopy azo-bis-isobutyronitrile adenosine-5’-monophosphate ampicillin charge-coupled device ciprofloxacin 7-carboxymethoxy-4methylcoumarin control polymer 2,4-dichlorophenoxyacetic acid danofloxacin dansyl-phenylalanine divinyl benzene 2,4-dichlorophenoxyacetic. LSP LSPR MAA MMA MeOH MIP MRL MS NIP NOR NPs PET PETIA PMT POAc PVA QD RAFT. acid methyl ester EDMA EDS. ethylene glycol dimethacrylate energy dispersive X-ray. SEM SERS. spectroscopy ELISA ENRO EtOH FB1 FlM FLU FQ FPIA FRET GlcA GlcN-6S GC HEMA HEPES. HPLC. IF KANA LOD. !. enzyme-linked immunosorbent assay enrofloxacin ethanol fumonisin B1 « fluorescent monomer » flumequine fluoroquinolone fluorescence polarization immunoassay Förster resonance energy. SPE SPR STRE TEM Tetraglyme TRIM UV 4-VPY Z-L-Phe. transfer β-D-glucuronic acid D-glucosamine-6-sulfate gas chromatography 2-hydroxyethyl methacrylate 2-[4-(2hydroxyethyl)piperazin-1yl]ethanesulfonic acid high-performance liquid chromatography imprinting factor kanamycin limit of detection. xi. localized surface plasmon localized surface plasmon resonance methacrylic acid methyl methacrylate methanol molecularly imprinted polymer maximum residue limit mass spectrometry non-imprinted polymer norfloxacin nanoparticles photoinduced electron transfer pentaerythritol triacrylate photomultiplier tube phenoxyacetic acid poly(vinyl alcohol) quantum dot reversible additionfragmentation chain transfer scanning electron microscopy surface-enhanced Raman spectroscopy solid phase extraction surface plasmon resonance streptomycin transmission electron microscopy tetraethylene glycol dimethyl ether trimethylolpropane trimethacrylate ultra-violet 4-vinyl pyridine N-(carbobenzyloxy)-Lphenylalanine.
(16) !. General1Introduction1 The research project CBI-PEM presented in this thesis was funded by the Regional Council of Picardy in France and co-funded by the European Union (FEDER). The work was performed from October 2010 to September 2013, in the UTC/CNRS Laboratory of Enzyme and Cell Engineering – Molecular Recognition and Catalysis, headed by Prof. Karsten Haupt at the Université de Technologie de Compiègne (UTC). This thesis was conducted under the supervision of Prof. Karsten Haupt and Dr. Bernadette Tse Sum Bui (UTC), and was coordinated to the Regional Council of Picardy by Dr. Victor Acha (Institut LaSalle Beauvais). The project CBI-PEM was initiated due to a pressing need for efficient food and environmental analysis and control. Everyday, we are confronted to various potentially toxic and endocrine disrupting compounds such as antibiotic residues, hormones, pesticides, bacterial and fungal toxins. In this project, we have specially focused on mycotoxins, toxins produced by fungi in a large variety of food (fruits, cereals, vegetables…). Mycotoxins are very resistant to biological, chemical and physical treatments, and can even remain in food after the disappearance of the fungi when cooking at high temperatures. Very toxic for humans and animals, most of them are mutagenic, teratogenic and/or carcinogenic such that nowadays mycotoxins have become a major concern for public health. Current methods used to detect mycotoxins are mostly chromatography coupled to mass spectrometry (HPLC, GC, LC/MS-MS, GC/MS-MS). Although these techniques are very sensitive, they are unfortunately time-consuming, expensive, and laborious, often necessitating specialized laboratory staff. Alternative methods employ biosensors (with immobilized antibodies) and ELISA (Enzyme-Linked Immunosorbent Assay). These methods are sensitive and much faster; however, serious problems of reproducibility and stability are encountered. In this context has emerged a real need for a new kind of sensor, which would be sensitive, fast, robust, stable, reliable but also portable and easy to handle, even for non-specialized people, thus making possible on-site monitoring. Hence, biomimetic sensors based on the use of molecularly imprinted polymers (MIPs) that are tailor-made synthetic receptors, constitute a very promising alternative to the existing sensing methods. The project CBI-PEM aimed to develop an innovative technology based on optical fibers and MIPs for the sensitive and rapid detection of mycotoxins, and more generally, for the detection and quantification of any biological analyte of interest. Fiber optic sensors are of particular interest as they allow the design of cheap and portable devices, whereas MIPs combine high specificity and selectivity with superior stability and robustness compared to biological recognition elements such as antibodies. In this thesis, we designed a new generation of MIP-based optical sensors that could be industrialized in the near future, and ready to use for sensing in the “real world”, for food safety, environmental and biomedical control, and even for household use. This project was performed for some specific parts with external collaborators: Dr. Olivier Soppera (Institut de Sciences des Matériaux de Mulhouse, France) for the optimization of MIP photostructuring on optical fibers, Dr. Paolo Bonomi and Dr. Marina Resmini (Queen Mary University. 1 !.
(17) ! of London, UK) for the synthesis of the naphthalimide-based monomer, and Dr. Jean-François Masson (Université de Montréal, Canada), for the gold films and the micro- and nanostructured gold arrays. The thesis is organized in four chapters: one bibliographic chapter and three results chapters. Chapter 1 provides a literature overview of molecularly imprinted polymers (history, development, synthesis, applications), with an outline on their applications as recognition elements in optical chemical sensors. Chapter 2 presents the development of intrinsic fluorescence fiber optic sensors carrying in-situ polymerized MIP microstructures as recognition elements. Initially, dansyl-L-phenylalanine was used as fluorescent model target, for the optimization of the material photostructuring, to get the best sensitivity of the sensor. Composite gold nanoparticle-MIP tips were synthesized in order to use the effect of noble metal signal enhancement to increase the sensitivity of the sensor. Finally we generated intrinsic fluorescent MIPs by using a naphthalimide-based signaling monomer, whose fluorescence increases upon binding with analyte. The sensor was applied for the detection of low concentrations of non-fluorescent analytes such as the herbicide 2,4-D, the mycotoxin citrinin and the sphingolipid D-erythro-sphingosine-1-phosphate. Chapter 3 reports the use of evanescent waves for the synthesis of molecularly imprinted polymers and for fiber optic sensing. A disposable, cheap and versatile evanescent wave fiber optic sensor was developed by coating a signaling fluorescent MIP on a 4-cm long polystyrene optical waveguide. The sensor could be applied for the detection of the herbicide 2,4-D and the mycotoxin citrinin. In parallel, the technique of evanescent-wave photopolymerization was used for the synthesis of signaling MIP microdots on gold films and gold nanostructured surfaces. This study will enable the future development of plasmonic MIP nanosensors.. ! Chapter 4 describes the development of a rapid, sensitive and economic sensing method for the direct detection of UV-excited fluorescent analytes in food and environmental samples. This sensing method is based on a fluorescence polarization assay using molecularly imprinted polymer nanoparticles. The technique was successfully applied for the detection of fluoroquinolone antibiotic residues. in. water. and. milk. samples. 2 !. below. their. maximum. residue. limit..
(18) !. .. General Introduction. 3 !. . ..
(19) Chapter(1 ( Molecularly*Imprinted*Polymers*and*Their* Applications*in*Optical*Sensing** A"Literature"Review".
(21) Chapter( 1:* Molecularly* Imprinted* Polymers* and* Their* Applications*in*Optical*Sensing*–*A"Literature"Review* I. Molecular imprinting I.1. The origin of molecular imprinting The first “molecular imprinting” effect, that is, a molecule leaving an imprint in a synthetic material, was observed in 1931 by the Russian chemist Polyakov, while he was studying porous silica matrices as new materials for chromatographic applications (Polyakov and Khim, 1931). In his study, polymerization of sodium silicate was performed with ammonium carbonate as gelating agent, and just before the drying step, an additive (benzene, toluene or xylene) was added in the medium. After drying of the silica gel, the additive was removed by washing with hot water. Subsequent adsorption studies revealed that the additive that had been added to the gel during the polymerization step showed higher adsorption on the silica gel, at least for benzene (Table 1.1). The adsorption was even higher over the two other additives in the case of benzene, as if the silica gel has demonstrated some sort of “molecular memory”. A few years later, this effect was explained by the structural changes induced by the additive in the silica matrix. Table 1.1. Rebinding on silica gels of different additives used during the preparation of the respective gels. Reproduced from Sellergren, 2000.. Adsorption on the silica gel (%) Gel prepared with. Benzene. Toluene. Xylene. Benzene. 87.5. 80.6. 80.1. Toluene. 88.5. 87.2. 86.7. Xylene. 75.1. 79. 68.3. Later, Linus Pauling proposed an interesting, although proven wrong, theory about the formation of antibodies (Pauling, 1940). He suggested that all antibodies had the same primary structure as normal globulin, and that the functional antibody was formed using the antigen as a template for the folding of the antibody's polypeptide chain, resulting in a chain configuration that is complementary to the antigen. This template-induced conformation could then explain the high selectivity of antibodies. He was even able to prove his theory: he precipitated globulins under denaturing conditions in the presence of an 'antigen', and then slowly removed the denaturing agent, leading to redissolution of the globulins. He then observed that the globulins exhibited selective binding of the antigen. Even though we know today that this theory about the formation of antibodies is wrong, this is the first example of 'bio-imprinting'. Similarly to the experiments carried out by Polyakov, Pauling applied this theory to an inorganic system, silica, and the results were reported by his student Dickey (Dickey, 1949). In this study, polymerization of sodium silicate was performed in the presence of methyl orange (and other alkyl orange dyes) used as the template. Subsequent adsorptions studies showed that the silica gel demonstrated selectivity for the dye that was present in the system during the polymerization, over other dyes. Furthermore, adsorption of the dye was also much higher on the corresponding “dye-imprinted” silica than on a “non-imprinted” silica gel (polymerized in absence of dye) (Table 1.2).. 6.
(22) ! !. Chapter 1: Molecularly Imprinted Polymers and Their Applications in Optical Sensing – A Literature Review. ! !. To explain this result, Morrison and co-workers proposed an “association mechanism” instead of the “footprint” or “imprint mechanism” (Morrison et al., 1959). In the “association mechanism”, the trapped dyes that remained after washing acted as “nucleation sites”, inducing the formation of complexes, which can explain the selectivity of the gel. Waksmundzki and co-workers performed extensive studies on the sorption of template to imprinted silicas combined with thermodynamic studies that led to the conclusion that the templates were adsorbed as multilayers to the silica. These results support the association mechanism proposed by the group of Morrison. However, later, Beckett and Youssef challenged the association mechanism theory with a study on quinine-selective silica (Beckett and Youssef, 1963). They showed that the selectivity of silica was suppressed when steam was forced through silica, or after treatment with dry organic solvents that did not remove the trapped molecules. These changes in selectivity are more likely to result from changes in the “footprint” structure, than from changes in the attractive forces of the trapped molecules. At the moment, most of the literature data seem to support the “footprint” mechanism, even if there is not enough evidence to refute definitely the association mechanism (Alexander, 2006). It also seems that the possibility of the two mechanisms both taking place has not been considered (Sellergren, 2000). Table 1.2. Relative adsorption of different dyes on silica gels: the amount adsorbed on the “imprinted” silica related to a “non-imprinted” silica gel. Reproduced from Sellergren, 2000.. Relative adsorption power Gel prepared with. Methyl orange. Ethyl orange. Propyl orange. Butyl orange. Methyl orange. 3.5. 1.6. 1.1. 1.1. Ethyl orange. 2.5. 9. 2.1. 2.2. Propyl orange. 2.3. 5. 20. 6. Butyl orange. 1.5. 2.8. 5. 15. During two decades, intensive research was done on molecular imprinting in silica, but it was only in 1972 that molecular imprinting in organic polymers appeared, thanks to the independent contributions of Klotz (Takagishi and Klotz, 1972) and Wulff (Wulff and Sarhan, 1972). Takagishi and Klotz reported the synthesis of a molecularly imprinted polymer consisting in a polyethyleneimine polymer bearing –SH groups for cross-linking via the formation of disulfide bridges from thiobutyrolactone monomers, and using methyl orange as the template. As a result, as expected, they observed that the MIP demonstrated higher adsorption capacity towards the methyl orange dye than the non-imprinted control polymer. In his work, Wulff introduced for the first time the notion of enantiospecificity induced by a 'molecular memory' of chemical interactions. He co-polymerized a template molecule functionalized with polymerizable vinyl groups with divinylbenzene (DVB), in a solvent so as to form a non-swellable macroporous polymer. To illustrate his idea, he chose as a model template the 2,3-O-pvinylphenylboronic ester of D-glyceric acid p-vinylanilide that was co-polymerized with DVB in acetonitrile. After polymerization, he could remove at most 50% of the D-glyceric acid by hydrolysis, leaving binding cavities with asymmetrically arranged functional groups, due to the chirality of the template (Figure 1.1). The polymer had the capacity to rebind the quantity of D-glyceric acid that was removed, and when reacted with D,L-glyceric acid, it showed selectivity for the D-enantiomer over the L-enantiomer, thus demonstrating enantiospecificity. Wulff observed finally that the polymer lost its binding properties when swollen, underlining the importance of the shape of the binding cavities in the molecular recognition process.. 7.
(23) ! !. Chapter 1: Molecularly Imprinted Polymers and Their Applications in Optical Sensing – A Literature Review. ! !. Figure 1.1. Principle of molecular imprinting via covalent interactions, as shown by Wulff et al. 1972. Reproduced from Andersson and Nicholls, 2000.. In the 1980s, Mosbach and co-workers proposed a new “template approach” that revolutionized the area of molecular imprinting. In his work, he synthesized highly cross-linked polymers containing monomers with chemical functional groups that were likely to interact with a template molecule via non-covalent bonds (i.e. ionic, hydrogen bonds), or the hydrophobic effect. The high cross-linking degree of the polymer enabled the formation of stable tri-dimensional binding sites complementary to the template. After removal of the template by washing with a solvent, the MIP was able to recognize and bind specifically the template, compared to a (though chemically identical) nonimprinted polymer (NIP) (Arshady and Mosbach, 1981). A few years later, similarly to the work of Wulff, Mosbach and co-workers imprinted the polymer with the D- or L-enantiomer of phenylalanine ethyl ester, and observed that, when incubated with a racemic mixture, the MIP showed selective binding of the enantiomer that had been used for imprinting. The synthesis of the phenylalanine ethyl ester-imprinted polymer was performed with p-vinylbenzoic acid as the functional monomer and DVB as the cross-linker. The molecular recognition process was based on ionic interactions between the template and the functional monomer (Andersson et al., 1984). During the early days, the great potential of MIPs as separation materials was demonstrated. However, in 1993 the group of Mosbach opened a new perspective for these materials, by showing that MIPs could also be used as antibody mimics. In a paper published in Nature (Vlatakis et al., 1993), they showed that a theophylline-imprinted polymer and a diazepam-imprinted polymer could bind respectively theophylline and diazepam in human serum with specificities and selectivities comparable to those of antibodies. This work provoked a significant raise of interest in the technique of molecular imprinting, as it opened a whole new range of applications and research perspectives for MIPs, which subsequently were termed 'plastic antibodies'.. 8.
(24) ! !. Chapter 1: Molecularly Imprinted Polymers and Their Applications in Optical Sensing – A Literature Review. ! !. I.2. Fundamentals of molecularly imprinted polymers I.2.1. The covalent approach As mentioned previously, the covalent approach for molecular imprinting in organic polymers was first introduced by Wulff in 1972, and later developed by Shea (Shea and Thompson, 1978). In this approach, the template molecule is covalently bonded by chemical reaction with functional monomers, followed by co-polymerization with an excess of cross-linking monomers. After polymerization, the template is removed by chemical cleavage (such as by hydrolysis), resulting in cavities in the polymer matrix that are complementary to the template molecule in terms of shape and chemical functionalities. Rebinding of the template takes place via the same covalent interactions. As demonstrated by Wulff and by Shea, the resulting MIP was able to distinguish between enantiomers when a chiral template was used, due to the local asymmetry of the binding sites. The advantage of this covalent approach is that the template/monomer complex is stoichiometric, avoiding non-specific binding by randomly distributed binding groups. Furthermore the bonds between template and monomers are very stable, resulting in a high yield in binding sites. The resulting MIP therefore shows high specificity and selectivity towards the analyte. However, this approach is not very versatile as not all imprinting targets can be derivatized so as to carry polymerizable moieties. Moreover, as the rebinding occurs via covalent bonding, the kinetics of this binding process may be slow. I.2.2. The non-covalent approach based on self-assembly As mentioned before, the non-covalent approach to molecular imprinting was for the first time described by Mosbach and co-workers in 1981, who aimed to apply the “biochemist’s” point of view to the “template-polymerization” introduced by Wulff. They called it the “host-guest polymerization”, and in this approach, the interactions between the template and the functional monomers are only based on non-covalent interactions, such as hydrogen bonds, ionic, hydrophobic or π−π stacking interactions, van der Waals forces, etc. The complex between template and functional monomers is formed by selfassembly, and the polymerization is carried out with an excess of cross-linkers, in order to give rigidity to the polymer matrix and preserve the shape of the binding cavities formed (Figure 1.2). Similarly to the covalent approach, rebinding of the analyte occurs via the same interactions.. Figure 1.2. Schematic representation of the molecular imprinting principle by self-assembly approach. a: functional monomers, b: cross-linkers; c: template; 1: assembly of the pre-polymerization complex template/functional monomers, 2: polymerization, 3: extraction of the template, 4: rebinding of the analyte.. 9.
(25) ! !. Chapter 1: Molecularly Imprinted Polymers and Their Applications in Optical Sensing – A Literature Review. ! !. The advantage of this approach is that it can make use of a large choice of functional monomers, and be applied to a vast range of target analytes. Moreover, the synthesis is quite straightforward, even for non-chemists, as the protocol simply consists in mixing template, functional and cross-linking monomers, a polymerization initiator and a solvent. After polymerization, the template is removed by solvent extraction. Given the relative simplicity of this protocol, the range of applications of these MIPs is quite vast, as they can be synthesized in various formats. Thus this approach is more versatile than the covalent approach. However, it is based on the equilibrium of the pre-polymerization complex, whose stability depends on the affinity constants between the template and the functional monomers. Moreover, in most cases, the functional monomers have to be used in excess with respect to the template (typically 4 times the amount of template or more), in order to shift the equilibrium towards the formation of the complex. Consequently, some functional groups are distributed randomly in the polymer, thus creating low-affinity binding sites that are source of nonspecific binding. The highest affinity sites define the specific binding of the MIP. As a result, the population of binding sites is often heterogeneous (Figure 1.3).. Figure 1.3. Schematic representation of the heterogeneity of the population of binding sites in a MIP: high affinity site in (A) macropore and (F) micropore, (B) lower affinity site in macropore, (C) trapped template, (D) highest affinity site with shape selectivity for the template, (E) embedded site. Reproduced from Zimmerman and Lemcoff, 2004.. However, despite these disadvantages, the non-covalent approach has been the most popular one, because of its flexibility and versatility. Moreover, the binding properties of a non-covalent MIP, can be optimized if one takes into account the complexity of the system, which is composed of numerous reactants (the template, the functional monomers, the cross-linker, the initiator, the solvent) and influenced by a number other external parameters (the temperature, the pressure, the reaction time, etc.). In the following sections, we will consider more in detail how to choose the suitable monomers, and we will also discuss the “stoichiometric” functional monomers first introduced by Wulff (Wulff and Knorr, 2002) that allow binding with the analyte at a 1:1 molar ratio. I.2.2.1. The functional monomers Molecular imprinting by self-assembly is based on the non-covalent interactions that occur between the template and the functional monomers. Thus the choice of the functional monomers is of great importance. The functional monomer should carry a chemical group that can interact with the chemical. 10.
(26) ! !. Chapter 1: Molecularly Imprinted Polymers and Their Applications in Optical Sensing – A Literature Review. ! !. groups of the template, and the interactions should be as strong as possible. For example, acidic functional monomers are generally chosen to interact with basic templates, and vice-versa. Among the acid monomers, the most popular one is methacrylic acid (MAA), as its carboxylic acid group is able to establish ionic interactions with basic chemical groups, such as amino groups, and hydrogen bonds as a donor or as an acceptor. MAA was used for example to imprint theophylline (Vlatakis et al., 1993) (Figure 1.4), and a great variety of other targets. Some examples are reported in Table 3.. Figure 1.4. Schematic representation of the synthesis of the theophylline-imprinted polymer. (a) Complex formation between the functional monomer MAA and the template theophylline in a solvent; (b) Polymerization in the presence of the cross-linker; (c) Extraction of the template, leaving the specific binding sites in the MIP matrix. Adapted from (Vlatakis et al., 1993).. Apart from MAA, some other acidic functional monomers have been used in the literature, including acrylic acid, 2-acrylamido-2-methyl-1-propanesulfonic acid, itaconic acid, vinylbenzoic acid, etc. (Table 1.3). Among the basic monomers, 4-vinylpyridine (4-VPY) is the most commonly used. In particular, 4-VPY interacts strongly with carboxylic acids by ionic interactions, but also with with compounds that possess an aromatic ring, since in this case, π−π stacking can occur (Haupt et al., 1998a). Some other basic functional monomers with examples of templates are also reported in Table 1.3. In some cases, a combination of acidic and basic monomers can give rise to an enhanced selectivity, such as the combination MAA/4-VPY used for a MIP against N-protected L-phenylalanine derivatives (Ramstroem et al., 1993). Indeed L-phenylalanine possesses a carboxylic acid function that interacts with 4-VPY and hydrogen bond moieties that interact with MAA. Finally neutral functional monomers can be used, sometimes in addition, if certain specific properties of the material are required. For example, the functional monomer 2-hydroxyethyl methacrylate (HEMA) is hydrophilic and is often used in order to render the MIP less hydrophobic, in particular as a co-functional monomer in combination with MAA (Dirion et al., 2003). Among the other examples that can be found in the literature, we can cite styrene, which is hydrophobic and can interact with hydrophobic compounds or form π−π interactions with aromatic rings; another example is acrylamide, which is hydrophilic, and hydrogen bonding and can interact for example with carboxylic acids as well as amide groups. (Haupt, 2003b).. 11.
(27) ! !. Chapter 1: Molecularly Imprinted Polymers and Their Applications in Optical Sensing – A Literature Review. ! !. Table 1.3. Examples of the most popular functional monomers used in the non-covalent approach, with some associated templates. Adapted from Alexander et al., 2006 and Sellergren, 2000.. Nature of. Functional monomers. Templates. References. monomers Methacrylic acid. Proton acceptors, H-bond. Vlatakis et al., 1993;. donors and acceptors. Rachkov et al., 1998; Tse. (theophylline, steroids,. Sum Bui et al., 2010; Spivak. nucleotide bases, peptides…). and Shea, 1998; Kempe, 1996. Acidic. Acrylic acid. Amino acids. Sellergren et al., 1985. 4-Vinyl benzoic acid. Amino acids. Andersson et al., 1984. Tricyclic aromatics. Dunkin et al., 1993. 2-(Trifluoromethyl)acrylic acid. Nicotine. Matsui et al., 1997. Itaconic acid. Drugs. Fischer et al., 1991. 4-Vinylpyridine. Carboxylic acids (amino acids,. Kempe et al., 1993; Haupt,. 2,4-D…). Dzgoev, et al., 1998. N,N-Diethylaminoethyl. Alcohols and polar templates. Levi et al., 1997; Tarbin and. methacrylate. (estrogenic compounds,. Sharman, 1999; De Smet et. chloramphenicol, fumonisin. al., 2009. 2-Acrylamido-2-methyl-1propanesulfonic acid. Basic. B1…). Allylamine. Sialic acid. Piletsky et al., 1996. Acrylamide. Carboxylic acids and amides. Yu and Mosbach, 1998. (N-protected amino acids). Neutral. 2-Hydroxyethyl methacrylate. Hydrophilic templates (cAMP,. Turkewitsch et al., 1998;. salicylic acid, enrofloxacin…). Sreenivasan, 1997; Qiao and Sun, 2010. Styrene. Hydrophobic or aromatic. Claude et al., 2008. templates (tamoxifen). With the above-mentioned weakly interacting monomers, in order to shift the equilibrium towards the formation of the pre-polymerization complex, an excess of functional monomers is used, typically a ratio of template:functional monomers of 1:4 or higher. However, this can result in high nonspecific binding and has to be modulated depending on the template. There should be at least the same number of functional monomers than chemical functionalities in the template. In order to eliminate this drawback, Wulff and co-workers developed for the first time monomers that formed stoichiometric non-covalent complexes with the template, thanks to association constants of Ka > 10 -1. 3. M . In this case no non-specific binding is produced since no excess of monomer is required (Wulff. 12.
(28) ! !. Chapter 1: Molecularly Imprinted Polymers and Their Applications in Optical Sensing – A Literature Review. ! !. and Knorr, 2002). For comparison, the association constants of hydrogen bonds and electrostatic interactions between carboxylic acids and basic nitrogen, and with additional hydrogen bonds are -1. respectively Ka = 1.7, 3.3 and 30 M , in acetonitrile. In their work, Wulff and co-workers synthesized a series of monomers containing an amidine group, which can interact strongly with carboxylic acids by a combination of electrostatic and bidendate hydrogen bonds. An example of monomer is N,N’-diethyl-4-vinyl-benzamidine that can interact strongly with carboxylates, phosphonates and phosphates, with an association constant of 3. -1. 6. -1. 5.10 M < Ka < 10 M (Figure 1.5).. Figure 1.5. Complex formed between the monomer N,N’-diethyl-4-vinyl-benzamidine and the carboxyl group of the template. Adapted from Wulff and Knorr, 2002.. Later, Hall and co-workers developed a series of urea-based vinyl monomers for the stoichiometric recognition of oxyanions (they chose as first model templates Z-D or L-glutamic acid) (Hall. et. al.,. 2005).. In. particular,. the. urea-based. monomer. 1-(4-vinylphenyl)-3-(3,5-. bis(trifluoromethyl)phenyl)urea was employed stoichiometrically with penicillin G (Urraca et al., 2006; Urraca et al., 2007) (Figure 1.6) and the fluoroquinolone enrofloxacin (Benito-Peña et al., 2008), to extract them from aqueous samples. Besides carboxylates, the urea-monomer was also able to bind tyrosine phosphorylated peptides (Emgenbroich et al., 2008) and sulfated protein fragments in aqueous media (Shinde et al., 2012).. Figure 1.6. Stoichiometric electrostatic interactions between the monomer 1-(4-vinylphenyl)-3-(3,5bis(trifluoromethyl)phenyl)urea and (A) penicillin G (Urraca et al., 2006; 2007), (B) tyrosine phosphorylated peptides (Emgenbroich et al., 2008) and (C) sulfated protein fragments in aqueous media (Shinde et al., 2012).. I.2.2.2. The cross-linker The nature and the ratio of the cross-linker are of special importance, as in molecular imprinting, the polymer network should be rigid enough to maintain the tri-dimensional conformation of the specific binding sites (Wulff, 1995). However, at the same time, the binding sites should be easily accessible to. 13.
(29) ! !. Chapter 1: Molecularly Imprinted Polymers and Their Applications in Optical Sensing – A Literature Review. ! !. the analyte, and for this reason, the cross-linking degree should not be too high (Wulff, 2002). Usually, the cross-linking degree of a MIP ranges from 70% to 90%. The most commonly used cross-linkers are DVB (divinylbenzene) and EDMA (ethylene glycol dimethacrylate), which are bifunctional (they contain two polymerizable groups). They are generally used in organic media because of their hydrophobicity (Sellergren, 2000). EDMA is particularly popular in molecular imprinting as it combines a flexible chain structure with the rigidity and the prochiral character of the methacrylate groups (Wulff et al., 1987; Alexander et al., 2006). Other cross-linkers possessing three polymerizable groups are also often used in MIPs, such as TRIM (trimethylolpropane trimethacrylate) and PETIA (pentaerythritol triacrylate), which were shown to convey better properties to the MIP in some cases, for example as chiral stationary phases in HPLC (Kempe, 1996). Even if interactions are to take place only between the template and the functional monomers, it has been reported that the cross-linker can interact with the template as well (Wulff et al., 1987; Olsson et al., 2012). A very interesting approach was introduced by Spivak and co-workers, who developed MIP containing a single cross-linking monomer, N,O-bismethacrylolyl ethanolamine (NOBE) (Figure 1.7). These MIPs were called “OMNiMIPs” (one monomer molecularly imprinted polymer) (Sibrian-Vasquez and Spivak, 2004). The advantage of this approach is to simplify the formulation of the MIP. NOBE possess an amide group that can interact with alcohols and carboxylic acid groups (but not with amines). The OMNiMIPs were compared with traditional MAA/EDMA MIPs as separation materials in HPLC. As a result, the OMNiMIPs showed improved results in terms of enantioselective recognition in organic media, and similar results in aqueous media, compared to the MAA/EDMA MIPs. The incorporation of another functional monomer into the NOBE cross-linked MIP interfered with the good recognition process between the analyte and NOBE, resulting in lower selectivity. Apart from that, choosing the right cross-linker can render the MIP more compatible with a certain environment. For example, PETIA is a hydrophilic monomer and is often used to impart water compatibility to the MIP (Manesiotis et al., 2009; Ambrosini et al., 2012). Amide-based cross-linkers, such as N,N’-methylene-bis-acrylamide, provide a more polar environment, and are thus interesting for the imprinting of polar templates that show poor solubility in organic solvents (Sellergren, 2000).. Figure 1.7. Synthesis of an OMNiMIP, with NOBE, 1 as single cross-linking monomer. Reproduced from Sibrian-Vasquez and Spivak, 2004.. I.2.2.3. The solvent The role of the solvent is to dissolve the reactants of the pre-polymerization mixture, but also to induce porosity in the polymer, so that the inner binding sites are accessible to the analyte. If a bad solvent (for the polymer chains) is used, macroporosity is created in the MIP during the polymerization through phase separation between the growing polymer chains and the solvent. In a good solvent, the chains. 14.
(30) ! !. Chapter 1: Molecularly Imprinted Polymers and Their Applications in Optical Sensing – A Literature Review. ! !. remain solvated and a microporous gel-like material is obtained. A solvent is good for the polymer chains if their solubility parameters are close or identical (Sellergren, 2000). Generally, MIPs show the best recognition properties in the solvent in which they are synthesized (Andersson, 1996). Indeed, in this case the MIP is solvated in the same manner (no swelling or shrinking of the polymer with respect to the situation after synthesis), and the accessibility and the geometry of the binding sites are preserved. Considering that the molecular recognition process is based on weak non-covalents bonds (mostly hydrogen bonds), an apolar and aprotic solvent is often the most suitable, such as toluene or chloroform (Vlatakis et al., 1993). Acetonitrile, which is aprotic and moderately polar, is also popular for the synthesis of MIPs (Spivak and Shea, 1998). However, for some MIP formulations, it is also possible to use polar and protic solvents such as methanol (Turkewitsch et al., 1998), or even a mixture of methanol/water (Haupt et al., 1998a). In the latter case, the 2,4-D MIP even showed good rebinding of 2,4-D in pure buffer, due to the combination of ionic and π−π interactions that occurred between the template 2,4-D and the functional monomer 4-VPY. However, for some applications, solvents with specific properties are required. For example, in the case of MIP films obtained by spin-coating (Schmidt et al., 2004; 2005), the use of pure solvents (toluene, chloroform) resulted in MIPs with no porosity and very low binding properties, probably because solvent evaporation occurred before the phase separation between the polymer chains and the solvent. The use of a solvent with lower vapor pressure, diethylene glycol dimethyl ether (diglyme) only led to moderately improved MIP properties. The best binding properties and the highest porosity were finally obtained with the MIP prepared with a mixture diglyme/poly(vinyl acetate) (PVAc). The presence of the linear polymer PVAc was expected to accelerate the process of phase separation through spinodal decomposition (rather than nucleation and growth). Another example is the use of triethylene glycol dimethyl ether (triglyme) at only 33% of the volume of the monomers, for the fabrication of holographic MIPs (Fuchs et al., 2013). In this case, a compromise had to be made because porosity is necessary to promote access of the analyte to the binding sites, while in diffractive structures, porosity leads to light scattering and loss of efficiency. Nonetheless, it is also possible to obtain MIPs with good binding properties without any solvent in the precursors solution. For example, Byrne and co-workers synthesized MIPs hydrogels as soft contact lenses for uses in ophthalmic drug delivery. The MIP formulations consisted of 5 mole% of cross-linking monomer and 95 mole% of functional monomers (92 mole% of HEMA and 3 mole% of a combination of other functional monomers) (Venkatesh et al., 2007; Tieppo et al., 2012). Thus no solvent was incorporated into the MIP formulation during the polymerization, and yet, the MIP contact lenses could be successfully applied for drug loading and in-vivo controlled release (Tieppo et al., 2012). I.2.3. The 'semi-covalent' approach The semi-covalent approach was first introduced by Sellergren and Andersson (Sellergren and Andersson, 1990) and allows combining the advantages of covalent and non-covalent imprinting. In this approach, the template is covalently bound to the functional monomers, resulting, after extraction of the template by chemical cleavage, in a homogeneous population of binding sites. However, the rebinding of the template takes place via non-covalent interactions, resulting in fast binding kinetics.. 15.
(31) ! !. Chapter 1: Molecularly Imprinted Polymers and Their Applications in Optical Sensing – A Literature Review. ! !. In the approach proposed by Sellergren and Andersson, the template is directly coupled to the 2. 1. monomer. As illustrated in Figure 1.8, the “monomer-template” M -propionyl-O -acryl-oyl-L-2-amino-34. (O -acrylol-4-hydroxyphenyl)-1-propanol was synthesized from L-2-amino-3-(4-hydroxyphenyl)-1propanol, and co-polymerized with the cross-linker DVB. Hydrolysis of the template moiety left binding sites with carboxylic acid groups as functional groups. The MIP was then incubated with p-amino-Lphenylalanine ethyl ester, resulting in binding of the amino acid to the functional groups of the MIP, via hydrogen bonds and electrostatic interactions. However, the problem of this approach is that noncovalent interactions occur at a longer distance than covalent interactions, which can result in a possible distortion of the binding site geometry.. Figure 1.8. Synthetic route of the semi-covalent approach proposed by Sellergren and Andersson. Adapted from Sellergren and Andersson, 1990.. In order to circumvent this drawback, Whitcombe and co-workers introduced the semi-covalent imprinting with the use of a sacrificial spacer (Whitcombe et al., 1995). As shown in Figure 1.9, they applied their approach to imprint cholesterol, through the use of the “monomer-template” cholesteryl(4vinyl)-phenyl carbonate. The “monomer-template” was obtained by attaching cholesterol with 4vinylphenol via a carbonyl spacer. After co-polymerization with the cross-linker EDMA, the cholesterol template was removed by hydrolysis, and the spacer was also extracted as CO2. Rebinding of cholesterol could now take place via hydrogen bonding between its hydroxyl group and the phenolic group in the binding site.. 16.
(32) ! !. Chapter 1: Molecularly Imprinted Polymers and Their Applications in Optical Sensing – A Literature Review. ! !. However, this strategy can be applied only when hydroxyl groups are involved. The big drawback of the semi-covalent approach, as with the covalent approach, is the limited number of templates to which it can be applied.. Figure 1.9. Synthetic route of the semi-covalent approach using a sacrificial spacer for the imprinting of cholesterol through the use of cholesteryl(4-vinyl)phenyl carbonate (1). Reproduced from Whitcombe et al., 1995.. I.2.4. Polymerization procedures for MIPs MIPs are generally prepared by free-radical polymerization, which is a versatile method to synthesize MIPs under various physical formats, such as bulk, nanoparticles, dispersion, or films. In the following sections, we will have an overview over bulk and precipitation polymerization techniques, which were used in this thesis to prepare MIPs. The other methods will be presented briefly, but will not be discussed in detail, as they were not used in this work. I.2.4.1. Bulk polymerization Bulk polymerization is the traditional way to obtain polymers. Monomers are polymerized in the presence of an initiator or a catalyst, and no dispersing media or additional reactants are required. In this case, the probability of undesired chain transfer reactions is minimized. Bulk polymerization is often used for achieving step-growth polymerizations, such as polycondensations and polyadditions. However it is not used in industry for chain-growth polymerization, because of the Trommsdorff (Trommsdorff et al., 1948) or Norrish-Smith effect (Norrish and Smith, 1942) (also called the “autoacceleration” effect). Briefly, bulk polymerization induces a local increase in the viscosity of the polymerizing system that slow the Brownian motion of the growing polymer chains and the termination reactions. However, small monomers can still diffuse through the polymerizing system, thus increasing the propagation rate, and also the reaction heat, which can result in an alteration of the polymer properties. For industrial applications, the need for heat dissipation is a drawback for using bulk polymerization for chain-growth reactions. In the case of MIPs, the presence of solvent is required in order to generate porosity in the polymer. Thus bulk polymerization of MIPs refers to a system where the volume of solvent generally constitutes 50% of the volume of the pre-polymerization mixture. After polymerization, the resulting. 17.
(33) ! !. Chapter 1: Molecularly Imprinted Polymers and Their Applications in Optical Sensing – A Literature Review. ! !. bulk monolith is ground and sieved to obtain irregularly shaped particles of appropriate size (typically 5-50 µm), which can be used for various applications such as separation materials in chromatography or solid-phase extraction. Until now, bulk polymerization still remains the most used procedure for MIP synthesis (Alexander et al., 2006). However, bulk polymerization possesses several drawbacks: the procedure is time-consuming and causes loss of material, and as mentioned before, it is not suitable for industrial applications (Poma et al., 2010). Moreover, some applications require specific formats of MIPs, such as nanoparticles, core-shell beads, thin layers, membranes... For these other physical formats of MIPs, other polymerization procedures are specially adapted (Haupt, 2003b). I.2.4.2. Precipitation polymerization Precipitation polymerization was first introduced by Ye and co-workers (Ye et al., 1999), to synthesize MIP nanoparticles for the recognition of estradiol and theophylline. The nanoparticles had an average diameter of 200 nm for the theophylline-MIP, and of 300 nm for the estradiol-MIP (Figure 1.10). This method is now widely used in the MIP field in order to synthesize nanoparticles as it is quite easy and straightforward, and does not require stabilizers or other additives. The approach is based on the use of a solvent, where the monomers are soluble but the resulting polymer is not. The solvent generally constitutes at least 90% of the volume of the prepolymerization mixture. Contrary to bulk polymerization, the final material is not obtained by coagulation of the polymer chains, but is formed when the polymer chains grow until being insoluble, thus forming a precipitate. Compared to bulk materials, MIP beads prepared by precipitation polymerization can show better molecular recognition properties (Jiang and Tong, 2004; Lai et al., 2007). Indeed they have higher surface-to-volume ratios, resulting in higher binding capacities and kinetics, and better accessibility to the binding sites (Poma et al., 2010). Due to their enhanced properties, their small size and their spherical shape, these MIP particles have found numerous applications, such as immunoassays (Surugiu et al., 2000), capillary electrochromatography (Schweitz et al., 2000), fluorescence polarization assays (Hunt et al., 2006), chemiluminescence imaging (Surugiu et al., 2001a,b), or sensing materials (Reimhult et al., 2008). However, the drawback of this approach is the high dilution of monomers (a few percent, w/w) required in order to obtain small beads, which can affect the strength of the interactions between template and monomers. This problem can be overcome by choosing a couple of templates and functional monomers that interact strongly enough to form a stable complex under these conditions. Moreover, the size, shape and binding properties of the MIP nanoparticles obtained with this technique are not always well controlled, as it depends on several parameters, such as the reactants, the initiation, the temperature, the reaction time, and most importantly, the properties of the solvent with respect to the polymer.. 18.
(34) ! !. Chapter 1: Molecularly Imprinted Polymers and Their Applications in Optical Sensing – A Literature Review. ! !. Figure 1.10. Scanning electron micrograph of estradiol-imprinted polymer particles obtained by precipitation polymerization, of an average size of 300 nm. Reproduced from Ye et al., 1999.. I.2.4.3. Heterogeneous synthesis procedures of MIPs Heterogeneous procedures are used to synthesize MIPs and allow controlling the heat of the reaction, the viscosity of the medium, but also the size of the polymer beads. Contrary to bulk and precipitation polymerizations, heterogeneous polymerizations take place in two-phase systems where the starting monomers and/or the resulting polymer are in the form of a fine dispersion in an immiscible liquid. In addition to the monomers, the solvent and the initiator, some additives are added to the prepolymerization mixture to emulsify the monomers, and/or stabilize the monomer droplets and the resulting polymer. These polymerization procedures allow the synthesis of spherical polymer particles with typical sizes ranging from about 50 nm to 1-2 mm or larger (Arshady, 1992). Below, the techniques of suspension and emulsion polymerizations will be described briefly. Suspension polymerization In this approach, the monomers are mechanically dispersed in the form of small droplets in a noncompatible liquid, usually water, and are polymerized using a monomer-soluble initiator (Odian, 2004). The monomers are kept in suspension by continuous agitation and the addition of non-ionic stabilizers, such as poly(vinyl) alcohol or methyl cellulose, which can prevent droplet coalescence. The polymerization is confined into monomer droplets, where the mechanism and kinetics of polymerization are equivalent to bulk polymerization. The parameters that can be used to control the particle size are the stirring rate, the ratio of reactants, stabilizers, and temperature. If required a porogen can be added to the monomer droplets in order to make the resulting particles porous. This approach can be used to synthesize particles of any size, but is most suitable for synthesizing particles of size ranging from 20 to 2000 µm. However the size polydispersity obtained with this method is high. Several examples of MIPs beads obtained by suspension polymerization in aqueous phases can be found in the literature (Flores et al., 2000). However, given that water can affect the interactions between the template and the functional monomers, water has been replaced as the continuous phase by other media such as perfluorocarbons (Mayes and Mosbach, 1996), liquid paraffine (Kempe and Kempe, 2004) or silicone oil (Wang et al., 1996).. 19.